Heteroatom substitution effects in spin crossover dinuclear complexes.
Zaiter, Samantha; Kirk, Charlotte; Taylor, Matthew; Klein, Y. Maximilian; Housecroft, Catherine E.; Sciortino, Natasha F.; Clements, John E.; Cooper, Richard I.; Kepert, Cameron J.; Neville, Suzanne M.; Dalton transactions (Cambridge, England : 2003) 48 (2019) 7337–7343; doi:10.1039/c8dt05010d

data_7700102
_publ_section_title
;
 Heteroatom substitution effects in spin crossover dinuclear complexes.
;
_journal_issue                   21
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              7337
_journal_page_last               7343
_journal_paper_doi               10.1039/c8dt05010d
_journal_volume                  48
_journal_year                    2019
_chemical_formula_moiety         'C39 H30 Fe2 N24 S9, 4(C H4 O)'
_chemical_formula_sum            'C43 H46 Fe2 N24 O4 S9'
_chemical_formula_weight         1363.28
_chemical_name_common            'thtrz-S 100 K'
_chemical_name_systematic        '[Fe2(NCS)4(thtrz)5].4MeOH'
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2019-03-06 deposited with the CCDC.    2019-03-11 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 108.665(4)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   20.9095(9)
_cell_length_b                   13.9867(4)
_cell_length_c                   21.1519(8)
_cell_measurement_reflns_used    10022
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      25.7
_cell_measurement_theta_min      2.32
_cell_volume                     5860.6(4)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_molecular_graphics    'POV-RAY, WebLab Viewer'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT (Sheldrick 2018)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.910
_diffrn_measurement_device_type  mirror
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1061
_diffrn_reflns_av_unetI/netI     0.1255
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.910
_diffrn_reflns_limit_h_max       28
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            40959
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.910
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.556
_diffrn_reflns_theta_min         2.913
_diffrn_source                   'SuperNova (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    0.880
_exptl_absorpt_correction_T_max  0.844
_exptl_absorpt_correction_T_min  0.779
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.545
_exptl_crystal_description       block
_exptl_crystal_F_000             2800
_exptl_crystal_size_max          0.300
_exptl_crystal_size_mid          0.300
_exptl_crystal_size_min          0.200
_platon_squeeze_details
;
TITL c2om_a.res in C2/c
CELL   20.9095   13.9867   21.1519     90.00    108.67     90.00
SPGR C2/c
C101 0.661 0.095 0.704 !       4.65 eA-3
C102 0.181 0.363 0.158 !       3.83 eA-3
C103 0.588 0.063 0.624 !       3.24 eA-3
C104 0.987 0.502 0.440 !       1.84 eA-3
C105 0.455 0.070 0.466 !       1.82 eA-3
C106 0.512 0.049 0.482 !       1.56 eA-3
C107 0.982 0.438 0.445 !       1.55 eA-3
C108 0.994 0.471 0.068 !       1.51 eA-3
C109 0.988 0.495 0.000 !       1.50 eA-3
Q110 0.816 0.436 0.372 !       1.33 eA-3
C111 0.018 0.466 0.483 !       1.32 eA-3
C112 0.889 0.453 0.418 !       1.25 eA-3
C113 0.053 0.490 0.047 !       1.19 eA-3
Q114 0.546 0.076 0.950 !       1.18 eA-3
Q115 0.176 0.309 0.182 !       1.12 eA-3
Q116 0.970 0.386 0.014 !       1.07 eA-3
Q117 0.797 0.018 0.626 !       1.05 eA-3
Q118 1.000 0.203 0.249 !       1.04 eA-3
Q119 0.844 0.286 0.361 !       1.03 eA-3
C120 0.062 0.471 0.015 !       1.03 eA-3
C121 0.029 0.488 0.926 !       1.00 eA-3
Q122 0.843 0.488 0.277 !       1.00 eA-3
Q123 0.376 0.437 0.842 !       0.97 eA-3
Q124 0.105 0.498 0.106 !       0.96 eA-3
Q125 0.893 0.345 0.952 !       0.96 eA-3
Q126 0.028 0.047 0.378 !       0.95 eA-3
Q127 0.846 0.338 0.406 !       0.95 eA-3
Q128 0.186 0.465 0.234 !       0.94 eA-3
Q129 0.498 0.032 0.156 !       0.94 eA-3
Q130 0.015 0.359 0.893 !       0.93 eA-3
Q131 0.814 0.032 0.745 !       0.92 eA-3
Q132 0.969 0.314 0.969 !       0.92 eA-3
Q133 0.361 0.028 0.362 !       0.92 eA-3
Q134 0.895 0.423 0.453 !       0.91 eA-3
Q135 0.561 0.393 0.735 !       0.91 eA-3
Q136 0.516 0.156 0.940 !       0.91 eA-3
Q137 0.843 0.171 0.333 !       0.91 eA-3
Q138 0.453 0.391 0.892 !       0.90 eA-3
Q139 0.988 0.219 0.375 !       0.89 eA-3
C140 0.544 0.055 0.465 !       0.89 eA-3
C141 0.939 0.410 0.426 !       0.89 eA-3
C142 0.092 0.483 0.563 !       0.89 eA-3
Q143 0.560 0.140 0.421 !       0.89 eA-3
Q144 0.172 0.047 0.173 !       0.88 eA-3
Q145 0.375 0.329 0.361 !       0.87 eA-3
Q146 0.111 0.236 0.406 !       0.87 eA-3
Q147 0.876 0.343 0.904 !       0.87 eA-3
Q148 0.138 0.063 0.264 !       0.87 eA-3
Q149 0.672 0.122 0.935 !       0.86 eA-3
Q150 0.078 0.483 0.220 !       0.86 eA-3
Q151 0.500 0.266 0.670 !       0.86 eA-3
Q152 0.285 0.078 0.827 !       0.85 eA-3
Q153 0.122 0.277 0.326 !       0.85 eA-3
Q154 0.095 0.449 0.451 !       0.85 eA-3
Q155 0.388 0.498 0.094 !       0.85 eA-3
Q156 0.797 0.013 0.170 !       0.85 eA-3
Q157 0.313 0.439 0.687 !       0.84 eA-3
Q158 0.310 0.180 0.893 !       0.84 eA-3
Q159 0.228 0.499 0.048 !       0.84 eA-3
Q160 0.953 0.184 0.017 !       0.84 eA-3
Q161 0.749 0.391 0.107 !       0.83 eA-3
Q162 0.828 0.219 0.280 !       0.83 eA-3
Q163 0.543 0.045 0.926 !       0.83 eA-3
Q164 0.252 0.283 0.406 !       0.82 eA-3
Q165 0.315 0.126 0.469 !       0.82 eA-3
Q166 0.357 0.029 0.034 !       0.82 eA-3
Q167 0.576 0.089 0.466 !       0.82 eA-3
Q168 0.296 0.323 0.667 !       0.82 eA-3
Q169 0.467 0.281 0.124 !       0.81 eA-3
Q170 0.265 0.249 0.451 !       0.81 eA-3
Q171 0.893 0.501 0.235 !       0.81 eA-3
Q172 0.434 0.283 0.015 !       0.81 eA-3
C173 0.472 0.059 0.408 !       0.81 eA-3
Q174 0.357 0.237 0.388 !       0.81 eA-3
Q175 0.431 0.091 0.111 !       0.81 eA-3
Q176 0.252 0.309 0.207 !       0.80 eA-3
Q177 0.921 0.280 0.093 !       0.80 eA-3
Q178 0.144 0.450 0.048 !       0.80 eA-3
Q179 0.717 0.407 0.889 !       0.80 eA-3
Q180 0.237 0.450 0.889 !       0.80 eA-3
Q181 0.768 0.422 0.375 !       0.80 eA-3
Q182 0.285 0.112 0.735 !       0.80 eA-3
Q183 0.236 0.442 0.063 !       0.80 eA-3
Q184 0.157 0.360 0.560 !       0.79 eA-3
Q185 0.735 0.438 0.124 !       0.79 eA-3
Q186 0.114 0.218 0.065 !       0.79 eA-3
Q187 0.203 0.331 0.564 !       0.79 eA-3
Q188 0.861 0.158 0.371 !       0.79 eA-3
Q189 0.156 0.141 0.326 !       0.78 eA-3
Q190 0.221 0.186 0.030 !       0.78 eA-3
Q191 0.330 0.359 0.576 !       0.78 eA-3
Q192 0.033 0.033 0.454 !       0.77 eA-3
C193 0.442 0.072 0.423 !       0.77 eA-3
Q194 0.920 0.011 0.249 !       0.77 eA-3
Q195 0.481 0.107 0.971 !       0.76 eA-3
Q196 0.546 0.470 0.488 !       0.76 eA-3
C197 0.557 0.027 0.489 !       0.76 eA-3
Q198 0.318 0.044 0.829 !       0.76 eA-3
Q199 0.093 0.188 0.029 !       0.75 eA-3
;
_refine_diff_density_max         0.379
_refine_diff_density_min         -0.335
_refine_diff_density_rms         0.084
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.953
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     354
_refine_ls_number_reflns         7475
_refine_ls_number_restraints     7
_refine_ls_restrained_S_all      0.954
_refine_ls_R_factor_all          0.1416
_refine_ls_R_factor_gt           0.0646
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0519P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1143
_refine_ls_wR_factor_ref         0.1349
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4101
_reflns_number_total             7475
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8dt05010d2.cif
_cod_data_source_block           1884825
_cod_database_code               7700102
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.778
_shelx_estimated_absorpt_t_max   0.844
_shelx_res_checksum              40229
_platon_squeeze_void_probe_radius 1.20